Solar cell A solar cell or photovoltaic cell is a device that converts light directly into electricity by the photovoltaic effect. Sometimes the term solar cell is reserved for devices intended specifically to capture energy from sunlight, while the term photovoltaic cell is used when the light source is unspecified. Assemblies of cells are used to make solar panels, solar modules, or photovoltaic arrays. Photovoltaics is the field of technology and research related to the application of solar cells in producing electricity for practical use. The energy generated this way is an example of solar energy (also called solar power).
A solar cell made from a monocrystalline silicon wafer
Contents [hide] • •
1 History Of Solar Cells 2 Three generations of solar cells o 2.1 First generation o 2.2 Second generation o 2.3 Third generation 3 High efficiency cells o 3.1 Record efficiencies 3.1.1 Multiple junction solar cells 3.1.2 Thin film solar cells 4 Applications and implementations 5 Theory o 5.1 Simple explanation o 5.2 Photogeneration of charge carriers o 5.3 Charge carrier separation o 5.4 The p-n junction o 5.5 Connection to an external load o 5.6 Equivalent circuit of a solar cell 5.6.1 Characteristic equation 188.8.131.52 Open-circuit voltage and short-circuit current 184.108.40.206 Effect of physical size 220.127.116.11 Cell temperature 18.104.22.168 Series resistance 22.214.171.124 Shunt resistance 126.96.36.199 Reverse saturation current 188.8.131.52 Ideality factor 6 Solar cell efficiency factors o 6.1 Energy conversion efficiency
6.2 Thermodynamic Efficiency Limit 6.3 Quantum efficiency 6.4 Maximum-power point 6.5 Fill factor 6.6 Comparison of energy conversion efficiencies 6.6.1 Watts peak 6.6.2 Solar cells and energy payback 7 Light-absorbing materials o 7.1 Bulk 7.1.1 Crystalline silicon o 7.2 Thin films 7.2.1 Cadmium telluride solar cell 7.2.2 Copper-Indium Selenide 7.2.3 Gallium arsenide (GaAs) multijunction 7.2.4 Light-absorbing dyes (DSSC) 7.2.5 Organic/polymer solar cells 7.2.6 Silicon Thin Films 184.108.40.206 Nanocrystalline solar cells 8 Concentrating photovoltaics (CPV) 9 Silicon solar cell device manufacture 10 Lifespan 11 Costs o 11.1 Slicing costs o 11.2 Low Cost Solar Cell 12 Current research on materials and devices o 12.1 Silicon processing o 12.2 Thin-film processing o 12.3 Metamorphic Multijunction Solar Cell o 12.4 Polymer processing o 12.5 Nanoparticle processing o 12.6 Transparent conductors o 12.7 Silicon wafer based solar cells o 12.8 Infrared solar cells o 12.9 UV Solar cells o 12.10 3-D solar cells o 12.11 Antireflective and all-angle coating o 12.12 Metamaterials o 12.13 Photovoltaic thermal hybrid 13 Validation, Certification and Manufacturers o 13.1 United States 14 See also 15 References
16 External links
o o o o o
• • • •
 History Of Solar Cells Main article: Timeline of solar cells The term "photovoltaic" comes from the Greek φῶς (phōs) meaning "light", and "voltaic", meaning electric, from the name of the Italian physicist Volta, after whom a unit of electrical potential, the volt, is named. The term "photo-voltaic" has been in use in English since 1849. The photovoltaic effect was first recognized in 1839 by French physicist A. E. Becquerel. However, it was not until 1883 that the first solar cell was built, by Charles Fritts, who coated the semiconductor selenium with an extremely thin layer of gold to form the junctions. The device was only around 1% efficient. Sven Ason Berglund had a number of patents concerning methods of increasing the capacity of these cells. Russell Ohl patented the modern junction semiconductor solar cell in 1946, which was discovered while working on the series of advances that would lead to the transistor. The modern age of solar power technology arrived in 1954 when Bell Laboratories, experimenting with semiconductors, accidentally found that silicon doped with certain impurities was very sensitive to light. Daryl Chapin, with Bell Labs colleagues Calvin Fuller and Gerald Pearson, invented the first practical device for converting sunlight into useful electrical power. This resulted in the production of the first practical solar cells with a sunlight energy conversion efficiency of around 6 percent.The solar battery was first demonstrated on April 25, 1954. The first spacecraft to use solar panels was the US satellite Vanguard 1, launched in March 1958 with solar cells made by Hoffman Electronics. This milestone created interest in producing and launching a geostationary communications satellite, in which solar energy would provide a viable power supply. This was a crucial development which stimulated funding from several governments into research for improved solar cells. In 1970 the first highly effective GaAs heterostructure solar cells were created by Zhores Alferov and his team in the USSR. Metal Organic Chemical Vapor Deposition (MOCVD, or OMCVD) production equipment was not developed until the early 1980s, limiting the ability of companies to manufacture the GaAs solar cell. In the United States, the first 17% efficient air mass zero (AM0) single-junction GaAs solar cells were manufactured in production quantities in 1988 by Applied Solar Energy Corporation (ASEC). The "dual junction" cell was accidentally produced in quantity by ASEC in 1989 as a result of the change from GaAs on GaAs substrates to GaAs on Germanium (Ge) substrates. The accidental doping of Ge with the GaAs buffer layer created higher open circuit voltages, demonstrating the potential of using the Ge substrate as another cell. As GaAs single-junction cells topped 19% AM0 production efficiency in 1993, ASEC developed the first dual junction cells for spacecraft use in the United States, with a starting efficiency of approximately 20%. These cells did not utilize the Ge as a second cell, but used another GaAs-based cell with different doping. Eventually GaAs dual junction cells reached production efficiencies of about 22%. Triple Junction solar cells
began with AM0 efficiencies of approximately 24% in 2000, 26% in 2002, 28% in 2005, and in 2007 have evolved to a 30% AM0 production efficiency, currently in qualification. Recent world record claims of efficiency for multiple junction solar cells are discussed in the Records section.
 Three generations of solar cells Solar Cells are classified into three generations which indicates the order of which each became important. At present there is concurrent research into all three generations while the first generation technologies are most highly represented in commercial production, accounting for 89.6% of 2007 production.  First generation Main articles: Crystalline silicon and Vacuum deposition First generation cells consist of large-area, high quality and single junction devices. First Generation technologies involve high energy and labor inputs which prevent any significant progress in reducing production costs. Single junction silicon devices are approaching the theoretical limiting efficiency of 31% and achieve an energy payback period of 5–7 years.  Second generation Main article: Thin-film cell Second generation materials have been developed to address energy requirements and production costs of solar cells. Alternative manufacturing techniques such as vapour deposition, electroplating, and use of Ultrasonic Nozzles are advantageous as they reduce high temperature processing significantly. It is commonly accepted that as manufacturing techniques evolve production costs will be dominated by constituent material requirements, whether this be a silicon substrate, or glass cover. The most successful second generation materials have been cadmium telluride (CdTe), copper indium gallium selenide, amorphous silicon and micromorphous silicon. These materials are applied in a thin film to a supporting substrate such as glass or ceramics, reducing material mass and therefore costs. These technologies do hold promise of higher conversion efficiencies, particularly CIGS-CIS, DSC and CdTe offers significantly cheaper production costs. Among major manufacturers there is certainly a trend toward second generation technologies, however commercialisation of these technologies has proven difficult. In 2007 First Solar produced 200 MW of CdTe solar cells making it the fifth largest producer of solar cells in 2007 and the first ever to reach the top 10 from production of second generation technologies alone. Wurth Solar commercialised its CIGS
technology in 2007 producing 15 MW. Nanosolar commercialised its CIGS technology in 2007 with a production capacity of 430 MW for 2008 in the USA and Germany.Honda, also began to commercialize their CIGS base solar panel in 2008. In 2007, CdTe production represented 8.9% of total market share, thin-film silicon 5.2% and CIGS 0.5%.  Third generation Main article: Third generation solar cell Third generation technologies aim to enhance poor electrical performance of second generation (thin-film technologies) while maintaining very low production costs. Current research is targeting conversion efficiencies of 30-60% while retaining low cost materials and manufacturing techniques. They can exceed the theoretical solar conversion efficiency limit for a single energy threshold material, that was calculated in 1961 by Shockley and Queisser as 31% under 1 sun illumination and 40.8% under the maximal artificial concentration of sunlight (46,200 suns, which makes the latter limit more difficult to approach than the former). There are a few approaches to achieving these high efficiencies including the use of Multijunction photovoltaic cells, concentration of the incident spectrum, the use of thermal generation by UV light to enhance voltage or carrier collection, or the use of the infrared spectrum for night-time operation.
 High efficiency cells High efficiency solar cells are a class of solar cell that can generate more electricity per incident solar power unit (watt/watt). Much of the industry is focused on the most cost efficient technologies in terms of cost per generated power. The two main strategies to bring down the cost of photovoltaic electricity are increasing the efficiency (as many of the costs scale with the area occupied per unit of generated power), and decreasing the cost of the solar cells per generated unit of power. The latter approach might come at the expense of reduced efficiency, so the overall cost of the photovoltaic electricity does not necessarily decrease by decreasing the cost of the solar cells. The challenge of increasing the photovoltaic efficiency is thus of great interest, both from the academic and economic points of view.
 Record efficiencies  Multiple junction solar cells The record for multiple junction solar cells is disputed. Teams led by the University of Delaware, the Fraunhofer Institute, and NREL all claim the world record title at 42.8, 41.1, and 40.8 percent, respectively. NREL claims that the other implementations
have not been put under standardized tests and, in the case of the University of Delaware project, represents only hypothetical efficiencies of a panel that has not been fully assembled. NREL claims it is one of only three laboratories in the world capable of conducting valid tests, although the Fraunhofer Institute is among those three facilities.  Thin film solar cells In 2002, the highest reported efficiency for solar cells based on thin films of CdTe is 18%, which was achieved by research at Sheffield Hallam University, although this has not been confirmed by an external test laboratory. The US national renewable energy research facility NREL achieved an efficiency of 19.9% for the solar cells based on copper indium gallium selenide thin films, also known as CIGS. These CIGS films have been grown by physical vapour deposition in a threestage co-evaporation process. In this process In, Ga and Se are evaporated in the first step; in the second step it is followed by Cu and Se co-evaporation and in the last step terminated by In, Ga and Se evaporation again.
 Applications and implementations
Polycrystaline PV cells laminated to backing material in a PV module Polycrystalline PV cells Main article: photovoltaic array Solar cells are often electrically connected and encapsulated as a module. PV modules often have a sheet of glass on the front (sun up) side, allowing light to pass while protecting the semiconductor wafers from the elements (rain, hail, etc.). Solar cells are also usually connected in series in modules, creating an additive voltage. Connecting cells in parallel will yield a higher current. Modules are then interconnected, in series or parallel, or both, to create an array with the desired peak DC voltage and current.
The power output of a solar array is measured in watts or kilowatts. In order to calculate the typical energy needs of the application, a measurement in watt-hours, kilowatt-hours or kilowatt-hours per day is often used. A common rule of thumb is that average power is equal to 20% of peak power, so that each peak kilowatt of solar array output power corresponds to energy production of 4.8 kWh per day (24 hours x 1kW x 20% = 4.8 kWh) To make practical use of the solar-generated energy, the electricity is most often fed into the electricity grid using inverters (grid-connected PV systems); in stand alone systems, batteries are used to store the energy that is not needed immediately. Solar cells can also be applied to other electronics devices to make it self power sustainable in the sun. There are solar cell phone chargers, solar bike light and solar camping lanterns that people can adopt for daily use.
 Theory See also: Electromotive force#Solar cell
 Simple explanation 1. Photons in sunlight hit the solar panel and are absorbed by semiconducting materials, such as silicon. 2. Electrons (negatively charged) are knocked loose from their atoms, allowing them to flow through the material to produce electricity. Due to the special composition of solar cells, the electrons are only allowed to move in a single direction. The complementary positive charges that are also created (like bubbles) are called holes and flow in the direction opposite of the electrons in a silicon solar panel. 3. An array of solar cells converts solar energy into a usable amount of direct current (DC) electricity.
 Photogeneration of charge carriers When a photon hits a piece of silicon, one of three things can happen: 1. the photon can pass straight through the silicon — this (generally) happens for lower energy photons, 2. the photon can reflect off the surface, 3. the photon can be absorbed by the silicon, if the photon energy is higher than the silicon band gap value. This generates an electron-hole pair and sometimes heat, depending on the band structure. When a photon is absorbed, its energy is given to an electron in the crystal lattice. Usually this electron is in the valence band, and is tightly bound in covalent bonds between neighboring atoms, and hence unable to move far. The energy given to it by the photon "excites" it into the conduction band, where it is free to move around within the
semiconductor. The covalent bond that the electron was previously a part of now has one fewer electron — this is known as a hole. The presence of a missing covalent bond allows the bonded electrons of neighboring atoms to move into the "hole," leaving another hole behind, and in this way a hole can move through the lattice. Thus, it can be said that photons absorbed in the semiconductor create mobile electron-hole pairs. A photon need only have greater energy than that of the band gap in order to excite an electron from the valence band into the conduction band. However, the solar frequency spectrum approximates a black body spectrum at ~6000 K, and as such, much of the solar radiation reaching the Earth is composed of photons with energies greater than the band gap of silicon. These higher energy photons will be absorbed by the solar cell, but the difference in energy between these photons and the silicon band gap is converted into heat (via lattice vibrations — called phonons) rather than into usable electrical energy.
 Charge carrier separation There are two main modes for charge carrier separation in a solar cell: 1. drift of carriers, driven by an electrostatic field established across the device 2. diffusion of carriers from zones of high carrier concentration to zones of low carrier concentration (following a gradient of electrochemical potential). In the widely used p-n junction solar cells, the dominant mode of charge carrier separation is by drift. However, in non-p-n-junction solar cells (typical of the third generation solar cell research such as dye and polymer solar cells), a general electrostatic field has been confirmed to be absent, and the dominant mode of separation is via charge carrier diffusion.
 The p-n junction Main articles: semiconductor and p-n junction The most commonly known solar cell is configured as a large-area p-n junction made from silicon. As a simplification, one can imagine bringing a layer of n-type silicon into direct contact with a layer of p-type silicon. In practice, p-n junctions of silicon solar cells are not made in this way, but rather, by diffusing an n-type dopant into one side of a ptype wafer (or vice versa). If a piece of p-type silicon is placed in intimate contact with a piece of n-type silicon, then a diffusion of electrons occurs from the region of high electron concentration (the ntype side of the junction) into the region of low electron concentration (p-type side of the junction). When the electrons diffuse across the p-n junction, they recombine with holes on the p-type side. The diffusion of carriers does not happen indefinitely however, because of an electric field which is created by the imbalance of charge immediately on either side of the junction which this diffusion creates. The electric field established across the p-n junction creates a diode that promotes charge flow, known as drift current,
that opposes and eventually balances out the diffusion of electron and holes. This region where electrons and holes have diffused across the junction is called the depletion region because it no longer contains any mobile charge carriers. It is also known as the "space charge region".
 Connection to an external load Ohmic metal-semiconductor contacts are made to both the n-type and p-type sides of the solar cell, and the electrodes connected to an external load. Electrons that are created on the n-type side, or have been "collected" by the junction and swept onto the n-type side, may travel through the wire, power the load, and continue through the wire until they reach the p-type semiconductor-metal contact. Here, they recombine with a hole that was either created as an electron-hole pair on the p-type side of the solar cell, or a hole that was swept across the junction from the n-type side after being created there. The voltage measured is equal to the difference in the quasi Fermi levels of the minority carriers ie. electrons in the p-type portion, and holes in the n-type portion.
 Equivalent circuit of a solar cell
The equivalent circuit of a solar cell The schematic symbol of a solar cell To understand the electronic behavior of a solar cell, it is useful to create a model which is electrically equivalent, and is based on discrete electrical components whose behavior is well known. An ideal solar cell may be modelled by a current source in parallel with a diode; in practice no solar cell is ideal, so a shunt resistance and a series resistance component are added to the model. The resulting equivalent circuit of a solar cell is shown on the left. Also shown, on the right, is the schematic representation of a solar cell for use in circuit diagrams.  Characteristic equation From the equivalent circuit it is evident that the current produced by the solar cell is equal to that produced by the current source, minus that which flows through the diode, minus that which flows through the shunt resistor:
I = IL − ID − ISH where
• • • •
I = output current (amperes) IL = photogenerated current (amperes) ID = diode current (amperes) ISH = shunt current (amperes)
The current through these elements is governed by the voltage across them:
Vj = V + IRS where • • • •
Vj = voltage across both diode and resistor RSH (volts) V = voltage across the output terminals (volts) I = output current (amperes) RS = series resistance (Ω)
By the Shockley diode equation, the current diverted through the diode is: 
where • • • • • •
I0 = reverse saturation current (amperes) n = diode ideality factor (1 for an ideal diode) q = elementary charge k = Boltzmann's constant T = absolute temperature For silicon at 25°C, volts.
By Ohm's law, the current diverted through the shunt resistor is: where •
RSH = shunt resistance (Ω)
Substituting these into the first equation produces the characteristic equation of a solar cell, which relates solar cell parameters to the output current and voltage: An alternative derivation produces an equation similar in appearance, but with V on the left-hand side. The two alternatives are identities; that is, they yield precisely the same results.
In principle, given a particular operating voltage V the equation may be solved to determine the operating current I at that voltage. However, because the equation involves I on both sides in a transcendental function the equation has no general analytical solution. However, even without a solution it is physically instructive. Furthermore, it is easily solved using numerical methods. (A general analytical solution to the equation is possible using Lambert's W function, but since Lambert's W generally itself must be solved numerically this is a technicality.) Since the parameters I0, n, RS, and RSH cannot be measured directly, the most common application of the characteristic equation is nonlinear regression to extract the values of these parameters on the basis of their combined effect on solar cell behavior.  Open-circuit voltage and short-circuit current
When the cell is operated at open circuit, I = 0 and the voltage across the output terminals is defined as the open-circuit voltage. Assuming the shunt resistance is high enough to neglect the final term of the characteristic equation, the open-circuit voltage VOC is: Similarly, when the cell is operated at short circuit, V = 0 and the current I through the terminals is defined as the short-circuit current. It can be shown that for a high-quality solar cell (low RS and I0, and high RSH) the short-circuit current ISC is:  Effect of physical size
The values of I0, RS, and RSH are dependent upon the physical size of the solar cell. In comparing otherwise identical cells, a cell with twice the surface area of another will, in principle, have double the I0 because it has twice the junction area across which current can leak. It will also have half the RS and RSH because it has twice the cross-sectional area through which current can flow. For this reason, the characteristic equation is frequently written in terms of current density, or current produced per unit cell area: where • • • • •
J = current density (amperes/cm2) JL = photogenerated current density (amperes/cm2) Jo= reverse saturation current density (amperes/cm2) rS = specific series resistance (Ω-cm2) rSH = specific shunt resistance (Ω-cm2)
This formulation has several advantages. One is that since cell characteristics are referenced to a common cross-sectional area they may be compared for cells of different physical dimensions. While this is of limited benefit in a manufacturing setting, where all
cells tend to be the same size, it is useful in research and in comparing cells between manufacturers. Another advantage is that the density equation naturally scales the parameter values to similar orders of magnitude, which can make numerical extraction of them simpler and more accurate even with naive solution methods. A practical limitation of this formulation is that as cell sizes shrink, certain parasitic effects grow in importance and can affect the extracted parameter values. For example, recombination and contamination of the junction tend to be greatest at the perimeter of the cell, so very small cells may exhibit higher values of J0 or lower values of rSH than larger cells that are otherwise identical. In such cases, comparisons between cells must be made cautiously and with these effects in mind.  Cell temperature
Effect of temperature on the current-voltage characteristics of a solar cell Temperature affects the characteristic equation in two ways: directly, via T in the exponential term, and indirectly via its effect on I0. (Strictly speaking, temperature affects all of the terms, but these two far more significantly than the others.) While increasing T reduces the magnitude of the exponent in the characteristic equation, the value of I0 increases in proportion to exp(T). The net effect is to reduce VOC (the open-circuit Voltage) linearly with increasing temperature. The magnitude of this reduction is inversely proportional to VOC; that is, cells with higher values of VOC suffer smaller reductions in voltage with increasing temperature. For most crystalline silicon solar cells the reduction is about 0.50%/°C, though the rate for the highest-efficiency crystalline silicon cells is around 0.35%/°C. By way of comparison, the rate for amorphous silicon solar cells is 0.20-0.30%/°C, depending on how the cell is made. The amount of photogenerated current IL increases slightly with increasing temperature because of an increase in the number of thermally generated carriers in the cell. This effect is slight, however: about 0.065%/°C for crystalline silicon cells and 0.09% for amorphous silicon cells. The overall effect of temperature on cell efficiency can be computed using these factors in combination with the characteristic equation. However, since the change in voltage is much stronger than the change in current, the overall effect on efficiency tends to be similar to that on voltage. Most crystalline silicon solar cells decline in efficiency by 0.50%/°C and most amorphous cells decline by 0.15-0.25%/°C. The figure to the right shows I-V curves that might typically be seen for a crystalline silicon solar cell at various temperatures.  Series resistance
Effect of series resistance on the current-voltage characteristics of a solar cell As series resistance increases, the voltage drop between the junction voltage and the terminal voltage becomes greater for the same flow of current. The result is that the current-controlled portion of the I-V curve begins to sag toward the origin, producing a significant decrease in the terminal voltage V and a slight reduction in ISC, the shortcircuit current. Very high values of RS will also produce a significant reduction in ISC; in these regimes, series resistance dominates and the behavior of the solar cell resembles that of a resistor. These effects are shown for crystalline silicon solar cells in the I-V curves displayed in the figure to the right.  Shunt resistance
Effect of shunt resistance on the current–voltage characteristics of a solar cell As shunt resistance decreases, the current diverted through the shunt resistor increases for a given level of junction voltage. The result is that the voltage-controlled portion of the IV curve begins to sag toward the origin, producing a significant decrease in the terminal current I and a slight reduction in VOC. Very low values of RSH will produce a significant reduction in VOC. Much as in the case of a high series resistance, a badly shunted solar cell will take on operating characteristics similar to those of a resistor. These effects are shown for crystalline silicon solar cells in the I-V curves displayed in the figure to the right.  Reverse saturation current
Effect of reverse saturation current on the current-voltage characteristics of a solar cell If one assumes infinite shunt resistance, the characteristic equation can be solved for VOC: Thus, an increase in I0 produces a reduction in VOC proportional to the inverse of the logarithm of the increase. This explains mathematically the reason for the reduction in VOC that accompanies increases in temperature described above. The effect of reverse saturation current on the I-V curve of a crystalline silicon solar cell are shown in the figure to the right. Physically, reverse saturation current is a measure of the "leakage" of carriers across the p-n junction in reverse bias. This leakage is a result of carrier
recombination in the neutral regions on either side of the junction.  Ideality factor
Effect of ideality factor on the current-voltage characteristics of a solar cell The ideality factor (also called the emissivity factor) is a fitting parameter that describes how closely the diode's behavior matches that predicted by theory, which assumes the p-n junction of the diode is an infinite plane and no recombination occurs within the spacecharge region. A perfect match to theory is indicated when n = 1. When recombination in the space-charge region dominate other recombination, however, n = 2. The effect of changing ideality factor independently of all other parameters is shown for a crystalline silicon solar cell in the I-V curves displayed in the figure to the right. Most solar cells, which are quite large compared to conventional diodes, well approximate an infinite plane and will usually exhibit near-ideal behavior under Standard Test Condition (). Under certain operating conditions, however, device operation may be dominated by recombination in the space-charge region. This is characterized by a significant increase in I0 as well as an increase in ideality factor to . The latter tends to increase solar cell output voltage while the former acts to erode it. The net effect, therefore, is a combination of the increase in voltage shown for increasing n in the figure to the right and the decrease in voltage shown for increasing I0 in the figure above. Typically, I0 is the more significant factor and the result is a reduction in voltage.
 Solar cell efficiency factors  Energy conversion efficiency Main article: Energy conversion efficiency
Dust often accumulates on the glass of solar panels seen here as black dots.
A solar cell's energy conversion efficiency (η, "eta"), is the percentage of power converted (from absorbed light to electrical energy) and collected, when a solar cell is connected to an electrical circuit. This term is calculated using the ratio of the maximum power point, Pm, divided by the input light irradiance (E, in W/m2) under standard test conditions (STC) and the surface area of the solar cell (Ac in m2). STC specifies a temperature of 25°C and an irradiance of 1000 W/m2 with an air mass 1.5 (AM1.5) spectrum. These correspond to the irradiance and spectrum of sunlight incident on a clear day upon a sun-facing 37°-tilted surface with the sun at an angle of 41.81° above the horizon. This condition approximately represents solar noon near the spring and autumn equinoxes in the continental United States with surface of the cell aimed directly at the sun. Thus, under these conditions a solar cell of 12% efficiency with a 100 cm2 (0.01 m2) surface area can be expected to produce approximately 1.2 watts of power. The losses of a solar cell may be broken down into reflectance losses, thermodynamic efficiency, recombination losses and resistive electrical loss. The overall efficiency is the product of each of these individual losses. Due to the difficulty in measuring these parameters directly, other parameters are measured instead: Thermodynamic Efficiency, Quantum Efficiency, VOC ratio, and Fill Factor. Reflectance losses are a portion of the Quantum Efficiency under "External Quantum Efficiency". Recombination losses make up a portion of the Quantum Efficiency, VOC ratio, and Fill Factor. Resistive losses are predominantly categorized under Fill Factor, but also make up minor portions of the Quantum Efficiency, VOC ratio. 
 Thermodynamic Efficiency Limit Solar cells operate as quantum energy conversion devices, and are therefore subject to the "Thermodynamic Efficiency Limit". Photons with an energy below the band gap of the absorber material cannot generate a hole-electron pair, and so their energy is not converted to useful output and only generates heat if absorbed. For photons with an energy above the band gap energy, only a fraction of the energy above the band gap can be converted to useful output. When a photon of greater energy is absorbed, the excess energy above the band gap is converted to kinetic energy of the carrier combination. The excess kinetic energy is converted to heat through phonon interactions as the kinetic energy of the carriers slows to equilibrium velocity. Solar cells with multiple band gap absorber materials are able to more efficiently convert the solar spectrum. By using multiple band gaps, the solar spectrum may be broken down into smaller bins where the thermodynamic efficiency limit is higher for each bin.
 Quantum efficiency
Main article: Quantum efficiency of a solar cell As described above, when a photon is absorbed by a solar cell it can produce a pair of free charge carriers, i.e. an electron-hole pair. One of the carriers (the minority carrier) may then be able to reach the p-n junction and contribute to the current produced by the solar cell; such a carrier is said to be collected. Alternatively, the carrier may give up its energy and once again become bound to an atom within the solar cell without being collected; this process is then called recombination since one electron and one hole recombine and thereby annihilate the associated free charge. The carriers that recombine do not contribute to the generation of electrical current. Quantum efficiency refers to the percentage of photons that are converted to electric current (i.e., collected carriers) when the cell is operated under short circuit conditions. External quantum efficiency (EQE) is the fraction of incident photons that are converted to electrical current, while internal quantum efficiency (IQE) is the fraction of absorbed photons that are converted to electrical current. Mathematically, internal quantum efficiency is related to external quantum efficiency by the reflectance (R) and the transmittance (T) of the solar cell by IQE = EQE / (1 − R − T). Please note that for a thick bulk Si solar cell T is approximately zero and is therefore in practical cases often neglected. Quantum efficiency should not be confused with energy conversion efficiency, as it does not convey information about the fraction of power that is converted by the solar cell. Furthermore, quantum efficiency is most usefully expressed as a spectral measurement (that is, as a function of photon wavelength or energy). Since some wavelengths are absorbed more effectively than others in most semiconductors, spectral measurements of quantum efficiency can yield valuable information about the quality of the semiconductor bulk and surfaces.
 Maximum-power point A solar cell may operate over a wide range of voltages (V) and currents (I). By increasing the resistive load on an irradiated cell continuously from zero (a short circuit) to a very high value (an open circuit) one can determine the maximum-power point, the point that maximizes V×I; that is, the load for which the cell can deliver maximum electrical power at that level of irradiation. (The output power is zero in both the short circuit and open circuit extremes). A high quality, monocrystalline silicon solar cell, at 25 °C cell temperature, may produce 0.60 volts open-circuit (Voc). The cell temperature in full sunlight, even with 25 °C air temperature, will probably be close to 45 °C, reducing the open-circuit voltage to 0.55 volts per cell. The voltage drops modestly, with this type of cell, until the short-circuit current is approached (Isc). Maximum power (with 45 °C cell temperature) is typically produced with 75% to 80% of the open-circuit voltage (0.43 volts in this case) and 90% of the short-circuit current. This output can be up to 70% of the Voc x Isc product. The short-circuit current (Isc) from a cell is nearly proportional to the illumination, while the
open-circuit voltage (Voc) may drop only 10% with a 80% drop in illumination. Lowerquality cells have a more rapid drop in voltage with increasing current and could produce only 1/2 Voc at 1/2 Isc. The usable power output could thus drop from 70% of the Voc x Isc product to 50% or even as little as 25%. Vendors who rate their solar cell "power" only as Voc x Isc, without giving load curves, can be seriously distorting their actual performance. The maximum power point of a photovoltaic varies with incident illumination. For systems large enough to justify the extra expense, a maximum power point tracker tracks the instantaneous power by continually measuring the voltage and current (and hence, power transfer), and uses this information to dynamically adjust the load so the maximum power is always transferred, regardless of the variation in lighting.
 Fill factor Another defining term in the overall behavior of a solar cell is the fill factor (FF). This is the ratio of the maximum power point divided by the open circuit voltage (Voc) and the short circuit current (Isc): The fill factor is directly affected by the values of the cells series and shunt resistance. Increasing the shunt resistance (Rsh) and decreasing the series resistance (Rs) will lead to higher fill factor, thus resulting in greater efficiency, and pushing the cells output power closer towards its theoretical maximum
 Comparison of energy conversion efficiencies Main article: Photovoltaics At this point, discussion of the different ways to calculate efficiency for space cells and terrestrial cells is necessary to alleviate confusion. In space, where there is no atmosphere, the spectrum of the sun is relatively unfiltered. However, on earth, with air filtering the incoming light, the solar spectrum changes. To account for the spectral differences, a system was devised to calculate this filtering effect. Simply, the filtering effect ranges from Air Mass 0 (AM0) in space, to approximately Air Mass 1.5 on earth. Multiplying the spectral differences by the quantum efficiency of the solar cell in question will yield the efficiency of the device. For example, a Silicon solar cell in space might have an efficiency of 14% at AM0, but have an efficiency of 16% on earth at AM 1.5. Terrestrial efficiencies typically are greater than space efficiencies. Solar cell efficiencies vary from 6% for amorphous silicon-based solar cells to 40.7% with multiple-junction research lab cells and 42.8% with multiple dies assembled into a hybrid package. Solar cell energy conversion efficiencies for commercially available multicrystalline Si solar cells are around 14-19%. The highest efficiency cells have not always been the most economical — for example a 30% efficient multijunction cell based on exotic materials such as gallium arsenide or indium selenide and produced in low
volume might well cost one hundred times as much as an 8% efficient amorphous silicon cell in mass production, while only delivering about four times the electrical power. However, there is a way to "boost" solar power. By increasing the light intensity, typically photogenerated carriers are increased, resulting in increased efficiency by up to 15%. These so-called "concentrator systems" have only begun to become costcompetitive as a result of the development of high efficiency GaAs cells. The increase in intensity is typically accomplished by using concentrating optics. A typical concentrator system may use a light intensity 6-400 times the sun, and increase the efficiency of a one sun GaAs cell from 31% at AM 1.5 to 35%. See Solar_cell#Concentrating photovoltaics (CPV) below and Concentrating solar power (CSP). A common method used to express economic costs of electricity-generating systems is to calculate a price per delivered kilowatt-hour (kWh). The solar cell efficiency in combination with the available irradiation has a major influence on the costs, but generally speaking the overall system efficiency is important. Using the commercially available solar cells (as of 2006) and system technology leads to system efficiencies between 5 and 19%. As of 2005, photovoltaic electricity generation costs ranged from ~0.60 US$/kWh (0.50 €/kWh) (central Europe) down to ~0.30 US$/kWh (0.25 €/kWh) in regions of high solar irradiation. This electricity is generally fed into the electrical grid on the customer's side of the meter. The cost can be compared to prevailing retail electric pricing (as of 2005), which varied from between 0.04 and 0.50 US$/kWh worldwide. (Note: in addition to solar irradiance profiles, these costs/kwh calculations will vary depending on assumptions for years of useful life of a system. Most c-Si panels are warranted for 25 years and should see 35+ years of useful life.) The chart at the right illustrates the various commercial large-area module energy conversion efficiencies and the best laboratory efficiencies obtained for various materials and technologies.
Reported timeline of solar cell energy conversion efficiencies (from National Renewable Energy Laboratory (USA)  Watts peak Main article: Watt-peak Since solar cell output power depends on multiple factors, such as the sun's incidence angle, for comparison purposes between different cells and panels, the measure of watts peak (Wp) is used. It is the output power under these conditions known as STC. The standard test conditions imply an insolation (solar irradiance) of 1000 W/m2, a solar reference spectrum AM (airmass) of 1.5 and a cell temperature 25°C  Solar cells and energy payback
Further information: Low-cost photovoltaic cell In the 1990s, when silicon cells were twice as thick, efficiencies were much lower than today and lifetimes were shorter, it may well have cost more energy to make a cell than it could generate in a lifetime. In the meantime, the technology has progressed significantly, and the energy payback time, defined as the recovery time required for generating the energy spent for manufacturing of the respective technical energy systems, of a modern photovoltaic module is typically from 1 to 4 years depending on the module type and location. Generally, thin film technologies - despite having comparatively low conversion efficiencies - achieve significantly shorter energy payback times than conventional systems (often < 1 year). With a typical lifetime of 20 to 30 years, this means that modern solar cells are net energy producers, i.e. they generate significantly more energy over their lifetime than the energy expended in producing them.
 Light-absorbing materials Main article: Absorption (electromagnetic radiation) All solar cells require a light absorbing material contained within the cell structure to absorb photons and generate electrons via the photovoltaic effect. The materials used in solar cells tend to have the property of preferentially absorbing the wavelengths of solar light that reach the earth surface; however, some solar cells are optimized for light absorption beyond Earth's atmosphere as well. Light absorbing materials can often be used in multiple physical configurations to take advantage of different light absorption and charge separation mechanisms. Photovoltaic panels are normally made of either silicon or thin-film cells: Many currently available solar cells are configured as bulk materials that are subsequently cut into wafers and treated in a "top-down" method of synthesis (silicon being the most prevalent bulk material). Other materials are configured as thin-films (inorganic layers, organic dyes, and organic polymers) that are deposited on supporting substrates, while a third group are configured as nanocrystals and used as quantum dots (electron-confined nanoparticles) embedded in a supporting matrix in a "bottom-up" approach. Silicon remains the only material that is well-researched in both bulk (also called wafer-based) and thin-film configurations.
 Bulk These bulk technologies are often referred to as wafer-based manufacturing. In other words, in each of these approaches, self-supporting wafers between 180 to
240 micrometers thick are processed and then soldered together to form a solar cell module.  Crystalline silicon Main articles: Crystalline silicon, Silicon, and list of silicon producers Basic structure of a silicon based solar cell and its working mechanism. By far, the most prevalent bulk material for solar cells is crystalline silicon (abbreviated as a group as c-Si), also known as "solar grade silicon". Bulk silicon is separated into multiple categories according to crystallinity and crystal size in the resulting ingot, ribbon, or wafer. 1. monocrystalline silicon (c-Si): often made using the Czochralski process. Singlecrystal wafer cells tend to be expensive, and because they are cut from cylindrical ingots, do not completely cover a square solar cell module without a substantial waste of refined silicon. Hence most c-Si panels have uncovered gaps at the four corners of the cells. 2. Poly- or multicrystalline silicon (poly-Si or mc-Si): made from cast square ingots — large blocks of molten silicon carefully cooled and solidified. Poly-Si cells are less expensive to produce than single crystal silicon cells, but are less efficient. US DOE data shows that there were a higher number of multicrystalline sales than monocrystalline silicon sales. Ribbon silicon is a type of multicrystalline silicon: it is formed by drawing flat thin films from molten silicon and results in a multicrystalline structure. These cells have lower efficiencies than poly-Si, but save on production costs due to a great reduction in silicon waste, as this approach does not require sawing from ingots.
 Thin films Main article: Thin film The various thin-film technologies currently being developed reduce the amount (or mass) of light absorbing material required in creating a solar cell. This can lead to reduced processing costs from that of bulk materials (in the case of silicon thin films) but also tends to reduce energy conversion efficiency (an average 7 to 10% efficiency), although many multi-layer thin films have efficiencies above those of bulk silicon wafers. They have become popular compared to wafer silicon due to lower costs and advantages including flexibility, lighter weights, and ease of integration.  Cadmium telluride solar cell
Main article: Cadmium telluride photovoltaics A cadmium telluride solar cell is a solar cell based on cadmium telluride, an efficient light-absorbing material for thin-film cells. Compared to other thin-film materials, CdTe is easier to deposit and more suitable for large-scale production. There has been much discussion of the toxicity of CdTe-based solar cells. The perception of the toxicity of CdTe is based on the toxicity of elemental cadmium, a heavy metal that is a cumulative poison. While the toxicity of CdTe is presently under debate, it has been shown that the release of cadmium to the atmosphere is impossible during normal operation of the cells and is unlikely during ﬁres in residential roofs. Furthermore, a square meter of CdTe contains approximately the same amount of Cd as a single C cell Nickel-cadmium battery, in a more stable and less soluble form.  Copper-Indium Selenide Main article: Copper indium gallium selenide solar cell Possible combinations of (I, III, VI) elements in the periodic table that have photovoltaic effect The materials based on CuInSe2 that are of interest for photovoltaic applications include several elements from groups I, III and VI in the periodic table. These semiconductors are especially attractive for thin film solar cell application because of their high optical absorption coefficients and versatile optical and electrical characteristics which can in principle be manipulated and tuned for a specific need in a given device. CIS is an abbreviation for general chalcopyrite films of copper indium selenide (CuInSe2), CIGS mentioned below is a variation of CIS. CIS films (no Ga) achieved greater than 14% efficiency. However, manufacturing costs of CIS solar cells at present are high when compared with amorphous silicon solar cells but continuing work is leading to more cost-effective production processes. The first large-scale production of CIS modules was started in 2006 in Germany by Wuerth Solar. Manufacturing techniques vary and include the use of Ultrasonic Nozzles for material deposition. Electro-Plating in other efficient technology to apply the CI(G)S layer. When gallium is substituted for some of the indium in CIS, the material is referred to as CIGS, or copper indium/gallium diselenide, a solid mixture of the semiconductors CuInSe2 and CuGaSe2, often abbreviated by the chemical formula CuInxGa(1-x)Se2. Unlike the conventional silicon based solar cell, which can be modelled as a simple p-n junction (see under semiconductor), these cells are best described by a more complex heterojunction model. The best efficiency of a thin-film solar cell as of March 2008 was 19.9% with CIGS absorber layer. Higher efficiencies (around 30%) can be obtained by using optics to concentrate the incident light or by using multi-junction tandem solar cells. The use of gallium increases the optical bandgap of the CIGS layer as compared to pure CIS, thus increasing the open-circuit voltage, but decreasing the short circuit current. In another point of view, gallium is added to replace indium due to gallium's
relative availability to indium. Approximately 70% of indium currently produced is used by the flat-screen monitor industry. However, the atomic ratio for Ga in the >19% efficient CIGS solar cells is ~7%, which corresponds to a bandgap of ~1.15 eV. CIGS solar cells with higher Ga amounts have lower efficiency. For example, CGS solar cells (which have a bandgap of ~1.7eV have a record efficiency of 9.5% for pure CGS and 10.2% for surface-modified CGS. Some investors in solar technology worry that production of CIGS cells will be limited by the availability of indium. Producing 2 GW of CIGS cells (roughly the amount of silicon cells produced in 2006) would use about 10% of the indium produced in 2004. For comparison, silicon solar cells used up 33% of the world's electronic grade silicon production in 2006. Se allows for better uniformity across the layer and so the number of recombination sites in the film are reduced which benefits the quantum efficiency and thus the conversion efficiency.  Gallium arsenide (GaAs) multijunction Main article: Multijunction photovoltaic cell High-efficiency multijunction cells were originally developed for special applications such as satellites and space exploration, but at present, their use in terrestrial concentrators might be the lowest cost alternative in terms of $/kWh and $/W. These multijunction cells consist of multiple thin films produced using Metalorganic vapour phase epitaxy. A triple-junction cell, for example, may consist of the semiconductors: GaAs, Ge, and GaInP2. Each type of semiconductor will have a characteristic band gap energy which, loosely speaking, causes it to absorb light most efficiently at a certain color, or more precisely, to absorb electromagnetic radiation over a portion of the spectrum. The semiconductors are carefully chosen to absorb nearly all of the solar spectrum, thus generating electricity from as much of the solar energy as possible. GaAs based multijunction devices are the most efficient solar cells to date, reaching a record high of 40.7% efficiency under solar concentration and laboratory conditions. This technology is currently being utilized in the Mars rover missions. Tandem solar cells based on monolithic, series connected, gallium indium phosphide (GaInP), gallium arsenide GaAs, and germanium Ge pn junctions, are seeing demand rapidly rise. In just the past 12 months (12/2006 - 12/2007), the cost of 4N gallium metal has risen from about $350 per kg to $680 per kg. Additionally, germanium metal prices have risen substantially to $1000–$1200 per kg this year. Those materials include gallium (4N, 6N and 7N Ga), arsenic (4N, 6N and 7N) and germanium, pyrolitic boron nitride (pBN) crucibles for growing crystals, and boron oxide, these products are critical to the entire substrate manufacturing industry.
Triple-junction GaAs solar cells were also being used as the power source of the Dutch four-time World Solar Challenge winners Nuna in 2005 and 2007, and also by the Dutch solar cars Solutra (2005) and Twente One (2007). The Dutch Radboud University Nijmegen set the record for thin film solar cell effiency using a single junction GaAs to 25.8% in August 2008 using only 4 µm thick GaAs layer which can be transferred from a wafer base to glass or plastic film.  Light-absorbing dyes (DSSC) Main article: Dye-sensitized solar cells Typically a ruthenium metalorganic dye (Ru-centered) is used as a monolayer of lightabsorbing material. The dye-sensitized solar cell depends on a mesoporous layer of nanoparticulate titanium dioxide to greatly amplify the surface area (200-300 m2/g TiO2, as compared to approximately 10 m2/g of flat single crystal). The photogenerated electrons from the light absorbing dye are passed on to the n-type TiO2, and the holes are passed to an electrolyte on the other side of the dye. The circuit is completed by a redox couple in the electrolyte, which can be liquid or solid. This type of cell allows a more flexible use of materials, and is typically manufactured by screen printing and/or use of Ultrasonic Nozzles, with the potential for lower processing costs than those used for bulk solar cells. However, the dyes in these cells also suffer from degradation under heat and UV light, and the cell casing is difficult to seal due to the solvents used in assembly. In spite of the above, this is a popular emerging technology with some commercial impact forecast within this decade.  Organic/polymer solar cells Organic solar cells and Polymer solar cells are built from thin films (typically 100 nm) of organic semiconductors such as polymers and small-molecule compounds like polyphenylene vinylene, copper phthalocyanine (a blue or green organic pigment) and carbon fullerenes and fullerene derivatives such as PCBM. Energy conversion efficiencies achieved to date using conductive polymers are low compared to inorganic materials. However, it improved quickly in the last few years and the highest NREL (National Renewable Energy Laboratory) certified efficiency has reached 6.77%. In addition, these cells could be beneficial for some applications where mechanical flexibility and disposability are important. These devices differ from inorganic semiconductor solar cells in that they do not rely on the large built-in electric field of a PN junction to separate the electrons and holes created when photons are absorbed. The active region of an organic device consists of two materials, one which acts as an electron donor and the other as an acceptor. When a photon is converted into an electron hole pair, typically in the donor material, the charges tend to remain bound in the form of an exciton, and are separated when the exciton diffuses to the donor-acceptor interface. The short exciton diffusion lengths of most
polymer systems tend to limit the efficiency of such devices. Nanostructured interfaces, sometimes in the form of bulk heterojunctions, can improve performance.  Silicon Thin Films Silicon thin-film cells are mainly deposited by chemical vapor deposition (typically plasma-enhanced (PE-CVD)) from silane gas and hydrogen gas. Depending on the deposition parameters, this can yield  : 1. Amorphous silicon (a-Si or a-Si:H) 2. Protocrystalline silicon or 3. Nanocrystalline silicon (nc-Si or nc-Si:H), also called microcrystalline silicon. It has been found that protocrystalline silicon with a low volume fraction of nanocrystalline silicon is optimal for high open circuit voltage. These types of silicon present dangling and twisted bonds, which results in deep defects (energy levels in the bandgap) as well as deformation of the valence and conduction bands (band tails). The solar cells made from these materials tend to have lower energy conversion efficiency than bulk silicon, but are also less expensive to produce. The quantum efficiency of thin film solar cells is also lower due to reduced number of collected charge carriers per incident photon. Amorphous silicon has a higher bandgap (1.7 eV) than crystalline silicon (c-Si) (1.1 eV), which means it absorbs the visible part of the solar spectrum more strongly than the infrared portion of the spectrum. As nc-Si has about the same bandgap as c-Si, the nc-Si and a-Si can advantageously be combined in thin layers, creating a layered cell called a tandem cell. The top cell in a-Si absorbs the visible light and leaves the infrared part of the spectrum for the bottom cell in nanocrystalline Si. Recently, solutions to overcome the limitations of thin-film crystalline silicon have been developed. Light trapping schemes where the weakly absorbed long wavelength light is obliquely coupled into the silicon and traverses the film several times can significantly enhance the absorption of sunlight in the thin silicon films. Thermal processing techniques can significantly enhance the crystal quality of the silicon and thereby lead to higher efficiencies of the final solar cells. A silicon thin film technology is being developed for building integrated photovoltaics (BIPV) in the form of semi-transparent solar cells which can be applied as window glazing. These cells function as window tinting while generating electricity.  Nanocrystalline solar cells
Main article: Nanocrystal solar cell These structures make use of some of the same thin-film light absorbing materials but are overlain as an extremely thin absorber on a supporting matrix of conductive polymer or
mesoporous metal oxide having a very high surface area to increase internal reflections (and hence increase the probability of light absorption). Using nanocrystals allows one to design architectures on the length scale of nanometers, the typical exciton diffusion length. In particular, single-nanocrystal ('channel') devices, an array of single p-n junctions between the electrodes and separated by a period of about a diffusion length, represent a new architecture for solar cells and potentially high efficiency.
 Concentrating photovoltaics (CPV) Concentrating photovoltaic systems use a large area of lenses or mirrors to focus sunlight on a small area of photovoltaic cells. High concentration means a hundred or more direct sunlight is focused. Most comercial producers are developing systems that concentrate between 400 and 1000 "suns". Nearly all concentration systems need a one axis or more often two axis tracking system for high precision, since most systems only use direct sunlight and need to aim at the sun with errors of less than 3 degrees. The primary attraction of CPV systems is their reduced usage of semiconducting material which is expensive and currently in short supply. Additionally, increasing the concentration ratio improves the performance of general photovoltaic materials. Despite the advantages of CPV technologies their application has been limited by the costs of focusing, sun tracking and cooling equipment. On October 25, 2006, the Australian federal government and the Victorian state government together with photovoltaic technology company Solar Systems announced a project using this technology, Solar power station in Victoria, planned to come online in 2008 and be completed by 2013. This plant, at 154 MW, would be ten times larger than the largest current photovoltaic plant in the world.
 Silicon solar cell device manufacture
Solar-powered scientific calculator Because solar cells are semiconductor devices, they share many of the same processing and manufacturing techniques as other semiconductor devices such as computer and
memory chips. However, the stringent requirements for cleanliness and quality control of semiconductor fabrication are a little more relaxed for solar cells. Most large-scale commercial solar cell factories today make screen printed poly-crystalline silicon solar cells. Single crystalline wafers which are used in the semiconductor industry can be made into excellent high efficiency solar cells, but they are generally considered to be too expensive for large-scale mass production. Poly-crystalline silicon wafers are made by wire-sawing block-cast silicon ingots into very thin (180 to 350 micrometer) slices or wafers. The wafers are usually lightly p-type doped. To make a solar cell from the wafer, a surface diffusion of n-type dopants is performed on the front side of the wafer. This forms a p-n junction a few hundred nanometers below the surface. Antireflection coatings, which increase the amount of light coupled into the solar cell, are typically next applied. Over the past decade, silicon nitride has gradually replaced titanium dioxide as the antireflection coating of choice because of its excellent surface passivation qualities (i.e., it prevents carrier recombination at the surface of the solar cell). It is typically applied in a layer several hundred nanometers thick using plasmaenhanced chemical vapor deposition (PECVD). Some solar cells have textured front surfaces that, like antireflection coatings, serve to increase the amount of light coupled into the cell. Such surfaces can usually only be formed on single-crystal silicon, though in recent years methods of forming them on multicrystalline silicon have been developed. The wafer then has a full area metal contact made on the back surface, and a grid-like metal contact made up of fine "fingers" and larger "busbars" are screen-printed onto the front surface using a silver paste. The rear contact is also formed by screen-printing a metal paste, typically aluminium. Usually this contact covers the entire rear side of the cell, though in some cell designs it is printed in a grid pattern. The paste is then fired at several hundred degrees Celsius to form metal electrodes in ohmic contact with the silicon. Some companies use an additional electro-plating step to increase the cell efficiency. After the metal contacts are made, the solar cells are interconnected in series (and/or parallel) by flat wires or metal ribbons, and assembled into modules or "solar panels". Solar panels have a sheet of tempered glass on the front, and a polymer encapsulation on the back. Tempered glass cannot be used with amorphous silicon cells because of the high temperatures during the deposition process.
 Lifespan Most commercially available solar cells are capable of producing electricity for at least twenty years without a significant decrease in efficiency.
 Costs Cost is established in cost-per-watt and in cost-per-watt in 24 hours for infrared capable photovoltaic cells.
 Slicing costs University of Utah engineers devised a new way to slice thin wafers of the chemical element germanium for use in the most efficient type of solar power cells. The new method should lower the cost of such cells by reducing the waste and breakage of the brittle semiconductor.
 Low Cost Solar Cell Main articles: Dye-sensitized solar cell and low-cost photovoltaic cell Dye-sensitized solar cell, and Luminescent solar concentrators are considered low-cost solar cells. This cell is extremely promising because it is made of low-cost materials and does not need elaborate apparatus to manufacture, so it can be made in a DIY way allowing more players to produce it than any other type of solar cell. In bulk it should be significantly less expensive than older solid-state cell designs. It can be engineered into flexible sheets. Although its conversion efficiency is less than the best thin film cells, its price/performance ratio should be high enough to allow them to compete with fossil fuel electrical generation.
 Current research on materials and devices See also: Timeline of solar cells There are currently many research groups active in the field of photovoltaics in universities and research institutions around the world. This research can be divided into three areas: making current technology solar cells cheaper and/or more efficient to effectively compete with other energy sources; developing new technologies based on new solar cell architectural designs; and developing new materials to serve as light absorbers and charge carriers.
 Silicon processing One way of reducing the cost is to develop cheaper methods of obtaining silicon that is sufficiently pure. Silicon is a very common element, but is normally bound in silica, or silica sand. Processing silica (SiO2) to produce silicon is a very high energy process - at current efficiencies, it takes one to two years for a conventional solar cell to generate as much energy as was used to make the silicon it contains. More energy efficient methods of synthesis are not only beneficial to the solar industry, but also to industries surrounding silicon technology as a whole. The current industrial production of silicon is via the reaction between carbon (charcoal) and silica at a temperature around 1700 degrees Celsius. In this process, known as
carbothermic reduction, each tonne of silicon (metallurgical grade, about 98% pure) is produced with the emission of about 1.5 tonnes of carbon dioxide. Solid silica can be directly converted (reduced) to pure silicon by electrolysis in a molten salt bath at a fairly mild temperature (800 to 900 degrees Celsius). While this new process is in principle the same as the FFC Cambridge Process which was first discovered in late 1996, the interesting laboratory finding is that such electrolytic silicon is in the form of porous silicon which turns readily into a fine powder, (with a particle size of a few micrometres), and may therefore offer new opportunities for development of solar cell technologies. Another approach is also to reduce the amount of silicon used and thus cost, is by micromachining wafers into very thin, virtually transparent layers that could be used as transparent architectural coverings. The technique involves taking a silicon wafer, typically 1 to 2 mm thick, and making a multitude of parallel, transverse slices across the wafer, creating a large number of slivers that have a thickness of 50 micrometres and a width equal to the thickness of the original wafer. These slices are rotated 90 degrees, so that the surfaces corresponding to the faces of the original wafer become the edges of the slivers. The result is to convert, for example, a 150 mm diameter, 2 mm-thick wafer having an exposed silicon surface area of about 175 cm2 per side into about 1000 slivers having dimensions of 100 mm × 2 mm × 0.1 mm, yielding a total exposed silicon surface area of about 2000 cm2 per side. As a result of this rotation, the electrical doping and contacts that were on the face of the wafer are located the edges of the sliver, rather than the front and rear as is the case with conventional wafer cells. This has the interesting effect of making the cell sensitive from both the front and rear of the cell (a property known as bifaciality). Using this technique, one silicon wafer is enough to build a 140 watt panel, compared to about 60 wafers needed for conventional modules of same power output.
 Thin-film processing Main article: Thin-film Thin-film photovoltaic cells can use less than 1% of the expensive raw material (silicon or other light absorbers) compared to wafer based solar cells, leading to a significant price drop per Watt peak capacity. There are many research groups around the world actively researching different thin-film approaches and/or materials. However, it remains to be seen if these solutions can achieve a similar market penetration as traditional bulk silicon solar modules. One particularly promising technology is crystalline silicon thin films on glass substrates. This technology combines the advantages of crystalline silicon as a solar cell material (abundance, non-toxicity, high efficiency,long-term stability) with the cost savings of using a thin-film approach.
Another interesting aspect of thin-film solar cells is the possibility to deposit the cells on all kind of materials, including flexible substrates (PET for example), which opens a new dimension for new applications.
 Metamorphic Multijunction Solar Cell The National Renewable Energy Laboratory won a R&D Magazine's R&D 100 Awards for its Metamorphic Multijunction Solar Cell, an ultra-light and flexible cell that converts solar energy with record efficiency. The ultra-light, highly efficient solar cell was developed at NREL and is being commercialized by Emcore Corp. of Albuquerque, N.M., in partnership with the Air Force Research Laboratories Space Vehicles Directorate at Kirtland Air Force Base in Albuquerque. It represents a new class of solar cells with clear advantages in performance, engineering design, operation and cost. For decades, conventional cells have featured wafers of semiconducting materials with similar crystalline structure. Their performance and cost effectiveness is constrained by growing the cells in an upright configuration. Meanwhile, the cells are rigid, heavy and thick with a bottom layer made of germanium. In the new method, the cell is grown upside down. These layers use high-energy materials with extremely high quality crystals, especially in the upper layers of the cell where most of the power is produced. Not all of the layers follow the lattice pattern of even atomic spacing. Instead, the cell includes a full range of atomic spacing, which allows for greater absorption and use of sunlight. The thick, rigid germanium layer is removed, reducing the cell's cost and 94% of its weight. By turning the conventional approach to cells on its head, the result is an ultra-light and flexible cell that also converts solar energy with record efficiency (40.8 percent under 326 suns concentration).
 Polymer processing The invention of conductive polymers (for which Alan Heeger, Alan G. MacDiarmid and Hideki Shirakawa were awarded a Nobel prize) may lead to the development of much cheaper cells that are based on inexpensive plastics. However, organic solar cells generally suffer from degradation upon exposure to UV light, and hence have lifetimes which are far too short to be viable. The bonds in the polymers, are always susceptible to breaking up when radiated with shorter wavelengths. Additionally, the conjugated double bond systems in the polymers which carry the charge, react more readily with light and oxygen. So most conductive polymers, being highly unsaturated and reactive, are highly sensitive to atmospheric moisture and oxidation, making commercial applications difficult.
 Nanoparticle processing
Experimental non-silicon solar panels can be made of quantum heterostructures, eg. carbon nanotubes or quantum dots, embedded in conductive polymers or mesoporous metal oxides. In addition, thin films of many of these materials on conventional silicon solar cells can increase the optical coupling efficiency into the silicon cell, thus boosting the overall efficiency. By varying the size of the quantum dots, the cells can be tuned to absorb different wavelengths. Although the research is still in its infancy, quantum dotmodified photovoltaics may be able to achieve up to 42 percent energy conversion efficiency due to multiple exciton generation (MEG).
 Transparent conductors Many new solar cells use transparent thin films that are also conductors of electrical charge. The dominant conductive thin films used in research now are transparent conductive oxides (abbreviated "TCO"), and include fluorine-doped tin oxide (SnO2:F, or "FTO"), doped zinc oxide (e.g.: ZnO:Al), and indium tin oxide (abbreviated "ITO"). These conductive films are also used in the LCD industry for flat panel displays. The dual function of a TCO allows light to pass through a substrate window to the active light absorbing material beneath, and also serves as an ohmic contact to transport photogenerated charge carriers away from that light absorbing material. The present TCO materials are effective for research, but perhaps are not yet optimized for large-scale photovoltaic production. They require very special deposition conditions at high vacuum, they can sometimes suffer from poor mechanical strength, and most have poor transmittance in the infrared portion of the spectrum (e.g.: ITO thin films can also be used as infrared filters in airplane windows). These factors make large-scale manufacturing more costly. A relatively new area has emerged using carbon nanotube networks as a transparent conductor for organic solar cells. Nanotube networks are flexible and can be deposited on surfaces a variety of ways. With some treatment, nanotube films can be highly transparent in the infrared, possibly enabling efficient low bandgap solar cells. Nanotube networks are p-type conductors, whereas traditional transparent conductors are exclusively n-type. The availability of a p-type transparent conductor could lead to new cell designs that simplify manufacturing and improve efficiency.
 Silicon wafer based solar cells Despite the numerous attempts at making better solar cells by using new and exotic materials, the reality is that the photovoltaics market is still dominated by silicon waferbased solar cells (first-generation solar cells). This means that most solar cell manufacturers are currently equipped to produce this type of solar cells. Consequently, a large body of research is being done all over the world to manufacture silicon waferbased solar cells at lower cost and to increase the conversion efficiencies without an exorbitant increase in production cost. The ultimate goal for both wafer-based and alternative photovoltaic concepts is to produce solar electricity at a cost comparable to currently market-dominant coal, natural gas, and nuclear power in order to make it the leading primary energy source. To achieve this it may be necessary to reduce the cost of
installed solar systems from currently about US$ 1.80 (for bulk Si technologies) to about US$ 0.50 per Watt peak power. Since a major part of the final cost of a traditional bulk silicon module is related to the high cost of solar grade poly silicon feedstock (about US$ 0.4/Watt peak) there exists substantial drive to make Si solar cells thinner (material savings) or to make solar cells from cheaper upgraded metallurgical silicon (so called "dirty Si"). IBM has a semiconductor wafer reclamation process that uses a specialized pattern removal technique to repurpose scrap semiconductor wafers to a form used to manufacture silicon-based solar panels. The new process was recently awarded the “2007 Most Valuable Pollution Prevention Award” from The National Pollution Prevention Roundtable (NPPR).
 Infrared solar cells Researchers at Idaho National Laboratory, along with partners at Microcontinuum Inc. (Cambridge, MA) and Patrick Pinhero of the University of Missouri, have devised an inexpensive way to produce plastic sheets containing billions of nanoantennas that collect heat energy generated by the sun and other sources, which garnered two 2007 Nano50 awards. The technology is the first step toward a solar energy collector that could be mass-produced on flexible materials. While methods to convert the energy into usable electricity still need to be developed, the sheets could one day be manufactured as lightweight "skins" that power everything from hybrid cars to computers and iPods with higher efficiency than traditional solar cells. The nanoantennas also have the potential to act as cooling devices that draw waste heat from buildings or electronics without using electricity. The nanoantennas target mid-infrared rays, which the Earth continuously radiates as heat after absorbing energy from the sun during the day; also double-sided nanoantenna sheets can harvest energy from different parts of the sun's spectrum. In contrast, traditional solar cells can only use visible light, rendering them idle after dark. Also Konarka is researching infrared light activated photovoltaics which would enable night-time power generation.
 UV Solar cells Japan's National Institute of Advanced Industrial Science and Technology (AIST) has succeeded in developing a transparent solar cell that uses ultraviolet (UV) light to generate electricity but allows visible light to pass through it. Most conventional solar cells use visible and infrared light to generate electricity. In contrast, the innovative new solar cell uses ultraviolet radiation. Used to replace conventional window glass, the installation surface area could be large, leading to potential uses that take advantage of the combined functions of power generation, lighting and temperature control. Also, easily fabricated PEDOT:PSS photovoltaic cells are ultraviolet light selective and sensitive.
 3-D solar cells Three-dimensional solar cells that capture nearly all of the light that strikes them and could boost the efficiency of photovoltaic (PV) systems while reducing their size, weight and mechanical complexity. The new 3D solar cells capture photons from sunlight using an array of miniature “tower” structures that resemble high-rise buildings in a city street grid.
 Antireflective and all-angle coating See also: Anti-reflective coating With a reflective coating, developed at RPI, the material absorbs 96.21 percent of incident sunlight. This gain in absorption was consistent across the entire spectrum of sunlight, from UV to visible light and infrared. Such a method tackles the problem of absorbing sunlight evenly and equally from all angles. The seven layers, each with a height of 50-100 nm, are made up of silicon dioxide and titanium dioxide nanorods positioned at an oblique angle. Each layer looks and functions similar to a dense forest where sunlight is "captured" between the trees. The nanorods were attached to a silicon substrate via chemical vapor disposition and the new coating can be affixed to nearly any photovoltaic materials for use in solar cells, including III-V multi-junction and cadmium telluride.
 Metamaterials Main article: Metamaterial Researchers at Duke University and Boston College have engineered a metamaterial that utilizes tiny geometric shapes to absorb both the electrical and magnetic properties of electromagnetic waves over a certain frequency range at a level that meets standards of scientific perfection. This results in the total absorption of light, turning it into heat, which can then create energy.
 Photovoltaic thermal hybrid Main article: Photovoltaic thermal hybrid solar collector Systems which combine Photovoltaic with thermal solar, the advantage of such a system is that the thermal solar part carries heat away and cools the PV cells, keeping temperature down lowers the resistance and improves the PV cell's efficiency.
 Validation, Certification and Manufacturers Further information: Silicon shortage
National Renewable Energy Laboratory tests and validates solar technologies. There are three reliable certifications of solar equipment: UL and IEEE (both U.S. standards) and IEC. Solar cells are manufactured primarily in Japan, China, Germany, Taiwan and the USA, though numerous other nations have or are acquiring significant solar cell production capacity. While technologies are constantly evolving toward higher efficiencies, the most effective cells for low cost electrical production are not necessarily those with the highest efficiency, but those with a balance between low-cost production and efficiency high enough to minimize area-related balance of systems cost. Those companies with large scale manufacturing technology for coating inexpensive substrates may, in fact, ultimately be the lowest cost net electricity producers, even with cell efficiencies that are lower than those of single-crystal technologies.
 United States Main article: Photovoltaics in the United States New manufacturing facilities for solar cells and modules in Massachusetts, Michigan, Ohio, Oregon, and Texas promise to add enough capacity to produce thousands of megawatts of solar devices per year within the next few years from 2008: In late September 2008, Sanyo Electric Company, Ltd. announced its decision to build a manufacturing plant for solar ingots and wafers (the building blocks for silicon solar cells) in Salem, Oregon. The plant will begin operating in October 2009 and will reach its full production capacity of 70 megawatts (MW) of solar wafers per year by April 2010. In early October 2008, First Solar, Inc. broke ground on an expansion of its Perrysburg, Ohio, facility that will add enough capacity to produce another 57 MW per year of solar modules at the facility, bringing its total capacity to roughly 192 MW per year. The company expects to complete construction early next year and reach full production by mid-2010. In mid-October 2008, SolarWorld AG opened a manufacturing plant in Hillsboro, Oregon, that is expected to produce 500 MW of solar cells per year when it reaches full production in 2011.
 See also Energy portal Sustainable development portal • • •
Amorphous silicon Anomalous photovoltaic effect Autonomous building
• • • • • • • • • • • • • • • • • • • • • • • • • • • • • • • •
Black silicon Energy development Fab Flexible photovoltaics Green technology Heat load Helianthos Kelvin probe force microscope Junction List of solar cell manufacturers Metallurgical grade silicon Microgeneration Maximum Power Point Tracking Nanotechnology Carbon nanotubes in photovoltaics Nanoantenna Nanowire Photodiode Photovore - (a robot – light-seeking, often light-powered) Printed electronics Renewable energy Roll-to-roll processing Semiconductor Shockley-Queisser limit Solar Engine Solar panel Solar roof Solar shingles Solar tracker Spectrophotometry Timeline of solar energy UV degradation
 References 1. ^ Alfred Smee (1849). Elements of Electro-Biology, or The Voltaic Mechanism of Man; of Electro-Pathology, Especially of the Nervous System.... London: Longman, Brown, Green, and Longmans. http://books.google.com/books?id=CU0EAAAAQAAJ&pg=PA15&dq=photovoltaic+date:0-1850. 2. ^ Light sensitive device 3. ^ D. M. Chapin, C. S. Fuller, and G. L. Pearson; J. Appl. Phys. 25, 676 (1954); 4. ^ Alferov, Zh. I., V. M. Andreev, M. B. Kagan, I. I. Protasov,and V. G. Trofim (1970). Fiz. Tekh. Poluprovodn 4: 2378. 5. ^ Nobel LecturePDF (4.62 MB) by Zhores Alferov, p.6
6. ^ a b Hirshman, William P; Hering, Garret; Schmela, Michael (March 2008), Market Survey: Cell & Module Production http://www.photon-magazine.com Photon International], p. 152 7. ^ a b c Green, Martin A (April 2002), "Third generation photovoltaics: solar cells for 2020 and beyond", Physica E: Low-dimensional Systems and Nanostructures 14 (1-2): 65–70, doi:10.1016/S1386-9477(02)00361-2 8. ^ a b c "What is the Energy Payback for PV?" (PDF). http://www.nrel.gov/docs/fy05osti/37322.pdf. Retrieved 2008-12-30. 9. ^ a b c Hirshman, William P; Hering, Garret; Schmela, Michael (March 2008), "Market Survey: Cell & Module Production 2007", Photon International: 140– 174 10. ^ Largest Solar Cell Factory Coming to Bay Area 11. ^ School of Photovoltaic and Renewable Energy Engineering, UNSW: Third Generation Photovoltaics (A better citation would be preferred here. You can help Wikipedia by providing one.)
12. ^ "UD-led team sets solar cell record, joins DuPont on $100 million project". http://www.udel.edu/PR/UDaily/2008/jul/solar072307.html. 13. ^ "World Record: 41.1% efficiency reached for multi-junction solar cells at Fraunhofer ISE". http://www.ise.fraunhofer.de/press-and-media/pdfs-zupresseinfos-englisch/2009/press-release-world-record-41.1-efficiency-reachedfor-multi-junction-solar-cells-at-fraunhofer-ise-pdf-file. 14. ^ "NREL Solar Cell Sets World Efficiency Record at 40.8 Percent". http://www.nrel.gov/news/press/2008/625.html. 15. ^ "NREL, DARPA Both Claim Record Solar Efficiency". http://www.greentechmedia.com/articles/nrel-darpa-both-claim-record-solarefficiency-1310.html. (A better citation would be preferred here. You can help Wikipedia by providing one.)
16. ^ Würfel, Peter (2005) . Physics of solar cells. Weinheim: Wiley-VCH. ISBN 3-527-40428-7. 17. ^ Eduardo Lorenzo (1994). Solar Electricity: Engineering of Photovoltaic Systems. Progensa. ISBN 8486505550. http://books.google.com/books?id=lYc53xZyxZQC&pg=PA78&ots=yzbQVvxR4 j&dq=equivalent+circuit+%22solar+cell%22&sig=UmtfSmrNuW75jf0b8cJEcSB Hyx0#PPA80,M1. 18. ^ Antonio Luque and Steven Hegedus (2003). Handbook of Photovoltaic Science and Engineering. John Wiley and Sons. ISBN 0471491969. http://books.google.com/books?id=ubCMhl_JjQC&pg=PT326&ots=JCxK40jS5E&dq=wp+%22watts+peak%22+defi nition&sig=DCn_ieGxE81wn1kBMtowVsnrEPQ. 19. ^ Jenny Nelson (2003). The Physics of Solar Cells. Imperial College Press. ISBN 978-1-86094-340-9. http://www.worldscibooks.com/physics/p276.html. 20. ^ exp represents the exponential function 21. ^ ASTM G 173-03, "Standard Tables for Reference Solar Spectral Irradiances: Direct Normal and Hemispherical on 37° Tilted Surface," ASTM International, 2003. 22. ^ "Solar Spectral Irradiance: Air Mass 1.5". National Renewable Energy Laboratory. http://rredc.nrel.gov/solar/spectra/am1.5/. Retrieved 2007-12-12.
23. ^ Generally, solar cells on the market today do not produce much electricity from ultraviolet light, instead it is either filtered out or absorbed by the cell, heating the cell. That heat is wasted energy and could even lead to overheating of the cell. This can result in damage to the cell due to lattice vibrations that create defects in the crystalline material. 24. ^ "Cheng-Hsiao Wu and Richard Williams" (1983). Limiting efficiencies for multiple energy-gap quantum devices. 54. American Institude of Physics, journal=J. Appl. Phys.. p. 6721. 25. ^ Jenny Nelson, "The Physics of Solar Cells," Chapter 1, 2003. URL: http://www.solarfreaks.com/download/file.php?id=281 26. ^ "UD-led team sets solar cell record, joins DuPont on $100 million project". udel.edu/PR/UDaily. 2007-07-24. http://www.udel.edu/PR/UDaily/2008/jul/solar072307.html. Retrieved 2007-0724. 27. ^ "Silicon Solar Cells with Screen-Printed Front Side Metallization Exceeding 19% Efficiency". http://www.ise.fhg.de/veroffentlichungen/22nd-europeanphotovoltaic-solar-energy-conference-and-exhibition-milano-italy-2007/siliconsolar-cells-with-screen-printed-front-side-metallization-exceeding-19efficiency/view. 28. ^ M. Ito, K. Kato, K. Komoto, et al. (2008). "A comparative study on cost and life-cycle analysis for 100 MW very large-scale PV (VLS-PV) systems in deserts using m-Si, a-Si, CdTe, and CIS modules". Progress in Photovoltaics: Research and Applications 16: 17–30. doi:10.1002/pip.770. 29. ^ K. L. Chopra, P. D. Paulson, and V. Dutta (2004). "Thin-film solar cells: An overview Progress in Photovoltaics". Research and Applications 12: 69–92. 30. ^ "Net Energy Analysis For Sustainable Energy Production From Silicon Based Solar Cells" (PDF). http://jupiter.clarion.edu/~jpearce/Papers/netenergy.pdf. Retrieved 2008-12-30. 31. ^ Corkish, Richard (1997). "Can Solar Cells Ever Recapture the Energy Invested in their Manufacture?". Solar Progress 18 (2): 16–17. http://www.csudh.edu/oliver/smt310-handouts/solarpan/pvpayback.htm. 32. ^ "String ribbon silicon solar cells with 17.8% efficiency". http://www.ece.gatech.edu/research/UCEP/papers/3world/STRING%20RIBBON %20SILICON%20SOLAR%20CELLS%20WITH%2017.8%25%20EFFICIENC Y.pdf. 33. ^ Fthenakis, Vasilis M. (August 2004), "Life cycle impact analysis of cadmium in CdTe PV production" (PDF), Renewable and Sustainable Energy Reviews 8: 303– 334, doi:10.1016/j.rser.2003.12.001, http://www.firstsolar.com/pdf/Brookhaven_Life_Cycle_Analysis.pdf 34. ^ Fthenakis, Vasilis M. (August 2004), "Life cycle impact analysis of cadmium in CdTe PV production" (PDF), Renewable and Sustainable Energy Reviews 8: 303– 334, doi:10.1016/j.rser.2003.12.001, http://www.firstsolar.com/pdf/Brookhaven_Life_Cycle_Analysis.pdf 35. ^ "NREL Sets New CIGS Thin Film Efficiency Record (March 30, 2008)". http://www.solarbuzz.com/news/NewsNATE50.htm. (A better citation would be preferred here. You can help Wikipedia by providing one.)
36. ^ "Indium". http://minerals.usgs.gov/minerals/pubs/commodity/indium/indiumcs06.pdf. 37. ^ Tuttle et el. (2005). Design Considerations and Implementation of Very-Large Scale Manufacturing of CIGS Solar Cells and Related Products. 20th European Photovoltaic Solar Energy Conference and Exhibition. (A better citation would be preferred here. You can help Wikipedia by providing one.)
38. ^ R. M. Swanson, "The Promise of Concentrators," Progress in Photovoltaics: Res. Appl. 8, pp. 93-111 (2000). 39. ^ http://www.spectrolab.com/DataSheets/TerCel/tercell.pdf 40. ^ Spectrolab - Frequently Asked Questions 41. ^ New world record for Nijmegen solar cell (dutch) 42. ^ http://www.foxbusiness.com/story/markets/industries/finance/solarmer-breaksworld-records-plastic-solar-technology/ Fox Business News 43. ^ Mayer, A et al. (2007). "Polymer-based solar cells". Materials Today 10 (11): 28. doi:10.1016/S1369-7021(07)70276-6. 44. ^ R.W. Collins, A.S. Ferlauto, G.M. Ferreira, C. Chen, J. Koh, R.J. Koval, Y. Lee, J.M. Pearce, and C. R. Wronski, Evolution of microstructure and phase in amorphous, protocrystalline, and microcrystalline silicon studied by real time spectroscopic ellipsometry, Solar Energy Materials and Solar Cells, 78(1-4), pp. 143-180, 2003. 45. ^ J. M. Pearce, N. Podraza, R. W. Collins, M.M. Al-Jassim, K.M. Jones, J. Deng, and C. R. Wronski Optimization of Open-Circuit Voltage in Amorphous Silicon Solar Cells with Mixed Phase (Amorphous + Nanocrystalline) p-Type Contacts of Low Nanocrystalline Content, Journal of Applied Physics, 101(11), 114301, 2007.http://me.queensu.ca/people/pearce/publications/documents/t14.pdf 46. ^ P. I. Widenborg and A. G. Aberle, "Polycrystalline silicon thin-film solar cells on AIT-textured glass superstrates," Advances in OptoElectronics, vol. 2007, September 2007. 47. ^ M. L. Terry, A. Straub, D. Inns, D. Y. Song, and A. G. Aberle, "Large opencircuit voltage improvement by rapid thermal annealing of evaporated solidphase-crystallized thin-film silicon solar cells on glass," Applied Physics Letters, vol. 86, p. 3, April 2005. 48. ^ http://www.nrel.gov/news/press/release.cfm/release_id=10 49. ^ http://www.nrel.gov/ncpv/new_in_cpv.html 50. ^ "World-leading mega scale station for Victoria" (PDF). Solar Systems Pty Ltd.. http://www.solarsystems.com.au/documents/SolarSystemsMediaRelease.pdf. 51. ^ Newswise Science News | Slicing Solar Power Costs with New Wafer-Cutting Method 52. ^ Nohira T, Yasuda K, Ito Y (2003). "Pinpoint and bulk electrochemical reduction of insulating silicon dioxide to silicon". Nat Mater 2 (6): 397–401. doi:10.1038/nmat900. PMID 12754498. 53. ^ Jin X, Gao P, Wang D, Hu X, Chen GZ (2004). "Electrochemical preparation of silicon and its alloys from solid oxides in molten calcium chloride". Angew. Chem. Int. Ed. Engl. 43 (6): 733–6. doi:10.1002/anie.200352786. PMID 14755706. 54. ^ "Sliver Technology Research at the Australian National University". http://solar.anu.edu.au/level_1/research/sliver.php.
55. ^ "Sliver Technology Research at The ANU". http://solar.anu.edu.au/level_1/research/sliver.php. Retrieved 2007-04-12. 56. ^ M. A. Green, "Consolidation of Thin-film Photovoltaic Technology: The Coming Decade of Opportunity," Progress in Photovoltaics: Research and Applications, vol. 14, pp. 383-392, August 2006. 57. ^ P. A. Basore, "CSG-1: Manufacturing a New Polycrystalline Silicon PV Technology," in Conference Record of the 2006 IEEE 4th World Conference on Photovoltaic Energy Conversion, Hawaii, 2006, pp. 2089-2093. 58. ^ M. A. Green, P. A. Basore, N. Chang, D. Clugston, R. Egan, R. Evans, D. Hogg, S. Jarnason, M. Keevers, P. Lasswell, J. O'Sullivan, U. Schubert, A. Turner, S. R. Wenham, and T. Young, "Crystalline silicon on glass (CSG) thin-film solar cell modules," Solar Energy, vol. 77, pp. 857-863, 2004. 59. ^ V. Terrazzoni-Daudrix, F.-J. Haug, C. Ballif, et al., "The European Project Flexcellence Roll to Roll Technology for the Production of High Efficiency Low Cost Thin Film Solar Cells," in Proc. of the 21st European Photovoltaic Solar Energy Conference, 4-8 September 2006, pp. 1669-1672. 60. ^ NREL: Feature Story - Photovoltaics Innovations Win 2 R&D 100 Awards 61. ^ Emcore Corporation | Fiber Optics · Solar Power 62. ^ "Peter Weiss". "Quantum-Dot Leap". Science News Online. http://google.com/url?sa=t&ct=res&cd=3&url=http%3A%2F%2Fwww.sciencene ws.org%2Farticles%2F20060603%2Fbob8.asp&ei=5KaURN_cH4jqwALo0JzTA w&sig2=EQhq943aU4Ybb3lE_-lJLA. Retrieved 2005-06-17. 63. ^ R. M. Swanson, "A Vision for Crystalline Silicon Photovoltaics," Progress in Photovoltaics: Research and Applications, vol. 14, pp. 443-453, August 2006. 64. ^ IBM Press room - 2007-10-30 IBM Pioneers Process to Turn Waste into Solar Energy - United States 65. ^ MicroContinuum, Inc 66. ^ http://www.inl.gov/ 67. ^ http://www.japanfs.org/db/database.cgi?cmd=dp&num=371&UserNum=&Pass= &AdminPass=&dp=data_e.html 68. ^ http://scitation.aip.org/getabs/servlet/GetabsServlet?prog=normal&id=APPLAB0 00083000011002097000001&idtype=cvips&gifs=yes 69. ^ 3D Solar Cells Boost Efficiency While Reducing Size, Weight and Complexity of Photovoltaic Arrays 70. ^ http://www.rpi.edu/futurechips/index.htm 71. ^ a b The world's most anti-reflective coating 72. ^ New Metamaterial Could Be A Perfect Solar Solution | EcoGeek - Clean Technology 73. ^ S.A. Kalogirou, Y. Tripanagnostopoulos (30 January, 2006). Hybrid PV/T solar systems for domestic hot water and electricity production 74. ^ Solar Cell Production Jumps 50 Percent in 2007 75. ^ EERE News: EERE Network News